|                      | SiO2   | KBS       | NABS   | NBS1      | NCS    |
| Na2O (mol%)          |        | 1         | 9.5    | 16        | 16     |
| K2O (mol%)           |        | 5         |        |           |        |
| MnO (mol%)           |        | Li2O:1    |        |           | CaO:10 |
| B2O3 (mol%)          |        | 19        | 15.2   | 10        |        |
| SiO2 (mol%)          | 100    | 72        | 72.4   | 74        | 74     |
| Al2O3 (mol%)         |        | 2         | 2.9    | -         |        |
| K (SiO2/B2O3)        |        | 3.8       | 4.8    | 7.4       |        |
| R (Na2O/B2O3)        |        | 0.37      | 0.63   | 1.6       |        |
| N4(B) from B-NMR     |        | 0.35 [27] | n.a.   | 0.82 [16] |        |
| N4(B) from model     |        | 0.37      | 0.63   | 0.94      |        |
| %(Si+B) with 1 NBO   | 0      | 0 (<3.5)  | 0 (<6) | 13.4      | 70     |
| Tg (degC) +-2degC    | 1130   | 523       | 585    | 550       | 530    |
| Tm (degC) +-2degC    | 2000   | 1450      | 1500   | 1450      | 1450   |
| a (10-6 K-1)+-5K-1   | 0.58   | 5.4       | n.a.   | 8.8       | 9.9    |
| r (g/cm3)+-0.01g/cm3 | 2.2    | 2.27      | 2.31   | 2.45      | 2.48   |
| Vm  (cm3/mol)        | 27.3   | 27.5      | 25.4   | 25.8      | 24.2   |
| OH  (mol%) d         | 0.0003 | 0.14      | 0.003  | 0.12      | 0.05   |
| E (GPa) +- 1 GPa     | 67.8   | 63.3      | 75     | 75.3      | 74.8   |
| Poisson ratio v      | 0.16   | n.a.      | 0.21   | 0.21      | 0.22   |
| pm [GPa]             | 14.06  | n.a.      | 15.85  | 15.85     | 15.68  |

Caption: Batch composition of glasses in the ternary alkali borosilicate glass system and their selected physical and structural properties including: glass transition temperature Tg , actual melting temperature Tm , thermal expansion coefficient a, density r, molar volume Vm , -OH content, hardness E, Poisson ratio n, and t maximum intrinsic pressure pm . N4, the fraction of [BO4]- groups of the total boron content, and the percentage of network-former entities containing one non-bridging oxygen atoms (NBOSi+B) are also included.

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "1", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "KBS"}
{"value": "9.5", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "NABS"}
{"value": "16", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "NBS1"}
{"value": "16", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "NCS"}
{"value": "5", "type": "Other"}
{"value": "19", "type": "Other"}
{"value": "15.2", "type": "Other"}
{"value": "10", "type": "Other"}
{"value": "100", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "SiO2"}
{"value": "72", "type": "Other"}
{"value": "72.4", "type": "Other"}
{"value": "74", "type": "Other"}
{"value": "74", "type": "Other"}
{"value": "2", "type": "Other"}
{"value": "2.9", "type": "Other"}
{"value": "3.8", "type": "Other"}
{"value": "4.8", "type": "Other"}
{"value": "7.4", "type": "Other"}
{"value": "0.37", "type": "Other"}
{"value": "0.63", "type": "Other"}
{"value": "1.6", "type": "Other"}
{"value": "0.35", "type": "Other"}
{"value": "0.82", "type": "Other"}
{"value": "0.37", "type": "Other"}
{"value": "0.63", "type": "Other"}
{"value": "0.94", "type": "Other"}
{"value": "0", "type": "Other"}
{"value": "0", "type": "Other"}
{"value": "0", "type": "Other"}
{"value": "13.4", "type": "Other"}
{"value": "70", "type": "Other"}
{"value": "1130", "type": "Other"}
{"value": "523", "type": "Other"}
{"value": "585", "type": "Other"}
{"value": "550", "type": "Other"}
{"value": "530", "type": "Other"}
{"value": "2000", "type": "Other"}
{"value": "1450", "type": "Other"}
{"value": "1500", "type": "Other"}
{"value": "1450", "type": "Other"}
{"value": "1450", "type": "Other"}
{"value": "0.58", "type": "Other"}
{"value": "5.4", "type": "Other"}
{"value": "8.8", "type": "Other"}
{"value": "9.9", "type": "Other"}
{"value": "2.2", "type": "Other"}
{"value": "2.27", "type": "Other"}
{"value": "2.31", "type": "Other"}
{"value": "2.45", "type": "Other"}
{"value": "2.48", "type": "Other"}
{"value": "27.3", "type": "Other"}
{"value": "27.5", "type": "Other"}
{"value": "25.4", "type": "Other"}
{"value": "25.8", "type": "Other"}
{"value": "24.2", "type": "Other"}
{"value": "0.0003", "type": "Glass_Compound_Amount", "constituent": "OH", "unit": "mol", "material": "SiO2"}
{"value": "0.14", "type": "Glass_Compound_Amount", "constituent": "OH", "unit": "mol", "material": "KBS"}
{"value": "0.003", "type": "Glass_Compound_Amount", "constituent": "OH", "unit": "mol", "material": "NABS"}
{"value": "0.12", "type": "Glass_Compound_Amount", "constituent": "OH", "unit": "mol", "material": "NBS1"}
{"value": "0.05", "type": "Glass_Compound_Amount", "constituent": "OH", "unit": "mol", "material": "NCS"}
{"value": "67.8", "type": "Other"}
{"value": "63.3", "type": "Other"}
{"value": "75", "type": "Other"}
{"value": "75.3", "type": "Other"}
{"value": "74.8", "type": "Other"}
{"value": "0.16", "type": "Other"}
{"value": "0.21", "type": "Other"}
{"value": "0.21", "type": "Other"}
{"value": "0.22", "type": "Other"}
{"value": "14.06", "type": "Other"}
{"value": "15.85", "type": "Other"}
{"value": "15.85", "type": "Other"}
{"value": "15.68", "type": "Other"}